1 NEW TECHNIQUE FOR SYNTHESIZING AMP: PRECIPITATION INSIDE AN ION-EXCHANGE RESIN AND ITS APPLICATION TO SEPARATION OF CESIUM FROM FISSION-PRODUCTS AND TO A 137 m Ba GENERATOR Harko Tamura Matsuda and Alcídio Abrãb PUBLICAÇÃO IPEN 13 IPEN-Pub-13 JUNHO/1980
2 CONSELHO DELIBERATIVO MEMBROS Dr. Luiz Cintra do Prado - Pratidantt Or. Edgardo Aavado Soara» Júnior - Vica-PraíWanta CONSELHEIROS Or. Hélclo ModMto da Cora Or. Ivano Humbert Marchai! Dr. Admar Carvallini Dr. Waldyr Muniz Oliva REPRESENTANTES Dr. Jacob Che-cot Paraira Riot Dr. Paolo Enrico Maria Zaghan SUPERINTENDENTS Hamani Augusto Lopat da Amorim
3 PUBLICAÇÃO IPEN 13 IPEN-Pub-13 JUNHO/1980 NEW TECHNIQUE FOR SYNTHESIZING AMP: PRECIPITATION INSIDE AN ION-EXCHANGE RESIN AND ITS APPLICATION TO SEPARATION OF CESIUM FROM FISSION-PRODUCTS AND TO A 137 m Ba GENERATOR Harko Tamura Matsuda and Alcidio Abrào CENTRO DE ENGENHARIA QUlKlICA CEQ-AUT 78 INSTITUTO DE PESQUISAS ENERGÉTICAS E NUCLEARES SAO PAULO - BRASIL
4 Sérit PUBLICAÇÃO I PEN INIS Categories and Descriptors B13 AMMONIUM COMPOUNDS: Synthesis CESIUM 137: Chromatography CESIUM 137: Ion exchange MOLYBDOPHOSPHATE: Synthesis
5 NEW TECHNIQUE FOR SYNTHESIZING AMP: PRECIPITATION INSIDE AN ION-EXCHANGE RESIN AND ITS APPLICATION TO SEPARATION OF CESIUM FROM FISSION-PRODUCTS AND TO A 137m Ba GENERATOR* Harko Tamura Matsuda and Alcidio Abrão ABSTRACT Thti work deal* with a new technique for synthesizing ammonium molybdophosphate, an inorganic ion exchanger which retains selectively cesium-137 from a mixture of fission products,. ' _. '.-' ~ Normally the use of this exchanger in column operation requires the use of asbestos, silica-gel or organic polymers at binder, due to in microcrystalline form. The new process employs a strong anionic resin, saturated with molybdate anions. This method enables the precipitation of ammonium molybdophosphate directly into the resinous structure by adding dihydrogen ammonium phosphate in 7,5M HNO3. lhe reactants maintened a; 60 C for a period of four hours has been found to be the opanum condition for a maximum yield of this compound (anionic resin-ammonium molybdophosphate - RAMP). The tests performed *or characterizing this compound are: molybdenum-phosphorus ratio determination, electronic absorption spectra, infra-red absorption spectra, reflection microscopy observations, electron probe micro-analysis and X-ray powder patterns. The mentioned analysis confirmed the presence of the ammonium molybdophosphate in the resinous structure, permitting, thereby, its use as a cation exchanger. RAMP showed a capacity of 0,48 me/g of dry material. The cesium retention studies were made using columns charged with RAMP compound. The behavior of some polivalent fission products was also studied. The RAMP columns was finally applied to separate cesium from irradiated uranium solutions. described. A method for the isolation of ' J7m Ba by successive elutions from R-AMP ( l37 Cs) exchanger (generator) is Several methods for cesium recovery have been proposed based mainly on precipitation, solvent extraction and ion-exchange. Ion-exchange on organic resins ' ' received a great deal of attention, but these exchangers are very susceptible to radiation damage and therefore are unsuitable for processing highly radioactive solutions. So, more recently, the emphasis has been given to mineral exchangers' 6 ' 9-1^' and particularly to the development of synthetic inorganic ion-exchangers. Among these compounds a number of insoluble hydroxides and metal salts' 7 ' 8 ' have been investigated to separate alkali ions. But the most selective exchange properties for cesium was observed with ammonium molybdophosphate' 1 ' 11 ' 12 ' 14 '. It has been known that ammonium ions in AMP are reversiblely exchangeable with alkali ions, specially cesium, and its saturation capacity is comparable to that of organic resins' 13 '. The main disadvantage is its microcrystalline form, making difficult its use for chromatographic ions separation on columns. 'Work presented to the Congress of American Chemical Society, Honolulu, April, 1-6, 1979, Section of Radioactive Waste Diposal V, (Fuel Reprocessing Topics). Aproved for publication in February 1980 Writing, orthography, concepts and final revision are of exclusive responsibility of ihc Authors
6 Column beds of this material would be impervious to fluids. Normally, the application of this exchanger in column operation requires the use of asbestos' 4-14 '. silica-gel' 2 ' 31 or organic polymers' 16 ' as binders. This papers describes a new technique tor synthesizing AMP to separate cesium-137 selectively from a mixture of fission-products. The process employs a strong anionic resin in molybdate form. This method enable* the precipitation of AMP directly into the resinous structure by adding dihydrogen ammonium phosphate. This exchanger was also applied to prepare a ' 37m Ba generator. Experimental Procedures Synthesis of AMP. Precipitation into Strong Anionic Resin as Binder (RAMP) The exchanger hereafter marked out as RAMP was prepared using macroreticular anionic resin, amberlite IRA-900, saturated with molybdate anions. To acertain the suitable conditions for AMP precipitation inside the resin structure, contact time between resin and NH 4 H 2 PO 4 solution and the temperature of precipitation were studied. The precipitation efficiency was verified by determining the retention percentage of cesium-137 on R-AMP. >37 Cs was analysed by gamma counting of MeV photopeak of its l37 Ba daughter. To a 15 ml of resin, 6g of dihydrogen ammonium phosphate dissolved in 30 ml of 7.5 M HNO 3 is added. The reactants maintened at 60 C for a period of four hours has been found to be the optimum conditions for a maximum yield. Cesium Retention on R-AMP In these experiments, 230 ml of tracer solution of cesium-137 (13300 cpm/ml specific activity total counting) in 2M HN0 3 was passed at a flow-rate of 0.5 ml.cm" 2.min" 1 through a glass chromatographic column (0.6cm I.D. and 25cm long) containing 4ml R-AMP compound. Cesium sorption on the R-AMP column is illustrated by a typical breakthrough curve shown in Figure 1. To recover the retained cesium from the column, several eluents containing different concentrations of HN0 3 and NH 4 NO 3 were tested (Figure 2). The best elution (95%) was achieved with 10M NH 4 NO 3-0.2M HNO 3. The exchange capacity of R-AMP was also determined using the same procedure and passing 100 ml of 0.2M potassium nitrate. It has been found to be 0.4 me/g of dry material. Characterization of the R-AMP Compound Various analysis to characterize the AMP precipitated into resinous structure were performed: molybdenum-phosphorous ratio determination This analysis was made after destroying the organic materials and determining Mo ai.d P by spectrophotometric methods. The medium value obtained for Mo:P ratio was near to 12:1, characteristic for the (NH 4 ) 3 PO4.12Mo0j compound. electronic absorption in the ultra-violet region was obtained using a dual L*an spectrophotometer. The sample was prepared spreading directly a mixture formed by powdered R-AMP and Canadian balsam diluted into xylene over a cellofane papei sheet Figure 3 shows the absorption peak at 310 nm which is characteristic of the phosphomolybdate yellow compound.
7 CL < c 3 o zi ç i I c I Q. o r i o O (D I
8 too Ehitnt (ml) Figure 2 - Elution curves of cesium from RAMP column. Column: 0.6 cm I D. x25cm, with 4 ml of RAMP; o 10M HN 4 NO 3-0 2MHNO 3 ; n 3M NH 4 NO 3 -cone. HNO 3 ; 3M NH«NO, - 3MHNO,
9 X nm) Figura 3 - Electronic adsorption spectra; R AMP; -.._.._ AMP powder; - in molybdate form; resin in nitrate form resin
10 - reflection microscopy observation The sample was prepared impregnating the compound over a hicitt support by compactation until 150 C is reached. After cooling, the sample was polished and the micrography was obtained using metailograph : microscopy. These micrographies showed the different patterns among resins in nitrate and molybdate forms and after AMP precipitation as well. electron probe microanalysis This method aliows to attain the P and Mo distribution inside the resinous structure by then characteristic radiations. PK a, and MoLa, (Figure 4) using the same sample used for the reflection microscopy analysis. Applications of RAMP Exchanger The RAMP column was applied to selectively retain cesium-137 from a mixture of fission-products as well as to prepare a barium-137m generator. in order to study the cesium-137 recovery from fission-products mixture the behavior of some long-lived polivalent products as ruthenium and rare-earths represented by europium was studied. Those elements showed a moderate retention on RAMP column from 2M HNOj medium and their decontamination was obtained by washing the column with 1M HNOj. In other experiments, 10 g U 3 O«pellets were irradiated at IPEN reactor (MTR type) for 6 months. After 180 days cooling time, the pellets were dissolved with HNOj. The solution was then adjusted to 3M HNOj and uranium extracted wilh TOP 30%-varsoi v/v. To minimize the interference of elements such as Zr-Nb. the reffinate was treated with oxalic acid to complex them. The resulting solution was percolated through a RAMP column to retain cesium-137. The final decontamination was obtained by washing a column with dilute H,CjO 4 and HF (Figures 5 and 6). Generator systems for barium-137m were developed based or the very high affinity of long-lived parent ' 17 Cs for AMP exchanger and weak retention of shortlived daughter IJ7m Ba The experiments were developed fixing the cesium-137 on RAMP column from nitric acid medium. The co'umn was then washed with 1M HNO 3 and after secular fquilibnum has been achieved, ' JTm Ba was easily eluted with 0.1N! or 0.3M HN0 3. The half-life determination of eluted IJ7m Ba showrc a low contamination of cesium-137 due to slight dissolution of the AMP. In order to determine the solubility of AMP and R-AMP in dilute acid medium, some experiments were done. These data revealed that the solubility increases with increasing contact time and it is higher at room temperature (~ 25 C) than at 0 C The solubility of the AMP alone is higher than the AMP reuined into the resin (RAMP). Based on those properties a reliable generator system was obtained using a column containing ' J 7 Cs charged on RAMP at the upper portion of the column over a small amount of free RAMP at the bo t ton to retain any cesium eluted with ' J7m Ba. Sucessive elutions made with a 0.1M - 0.3M HNOj at ~ 10 C gave IJ7m Ba completely free from the parent. It is recomended to keep the generator column inside a normal refrigerator (~ 10"CI whpn not in use. Conclusion Several AMP precipitation experiments on macroreticular anionic resin allowed to conclude that the best condition to synthesize this exchanger is at 60 C with four hours reactants contact time, the maximum yield of RAMP beinq attained. Analysis performed to characterize this exchanger confirmed the presence of AMP into the resinous structure, permitting thereby its use as cation exchanger. The R AMP showed a capacity of 0.4 me/g of dry material.
11 t r 44» e 41* 40* Figura 4 - Molybdenum and phosphorous charactcrrstic radiation-,»f R AMP compound
12 «o > o s i I! ->-..-..;.!_.. JÜH_.._ Figur» 6 - Gammaray ip»ctrj showing cesium 137 retention from irradisttd uranium lolution on RAMP column. G«(Li) dttactor; irradiated U solution 1 ml x 1); effluent' 1 ml(x 1); -.,-.,- charged R-AMP-2ml (x4)
13 V SÉ CM $ e o o Gamma Cntray(K«V) Figure 6 Gamma-ray spectrum of radiochermca/ly pure ' 3 7 Cs separated directly from an irradiated uranium solution with the aid of R-AMP column. Gel Li) detector
14 10 The RAMP is being sucessfully applied for the selective retention of cesium-137 from a mixture of fission-products. Among these, only ' s Zr- 95 Nb showed an appreciable retention on RAMP column but they were easily decontamined using oxalic or hydrofluoric acid as complexing agents. set up. Using a RAMP ( l37 Cs) column a reliable l37m Ba generator for many sucessive elutions was RESUMO Apresenta-se ne*to trabalho uma nova técnica de preparação de fosfomolibdato de amònio, um trocador inorgânico útil à rutenção seletiva de césio-137 de produtos de fissão. Devido a sua estrutura microcristalina, a utilização deste trocador em operações de coluna requer, normalmente, o uso de suportes como asbestos, silica-gel e polímeros orgânicos. O novo processo consiste no emprego de uma resina aniònica forte na forma molibdato, permitindo a precipitação de fosfomolibdato de amònio no interior do grão, mediante a adição de fosfato monobásico de amônio em ácido nítrico 7,5M. Obteve-se a melhor precipitação à temperatura de 60 C com um tempo de contacto de 4 horas, utilizando-se como suporte resina aniònica forte macroreticular, Amberlite IRA-900. O trocador formado nestas condições apresentou uma capacidade de troca de 0,48 me/g e 100% de retenção de césio-137 de soluções 2M em HN0 3. Obtido o trocador num suporte compatível com o seu emprego em colunas cromatográficas, realizaram-se algumas análises de caracterização do composto: determinação da relação Mo:P, espectro eletrônico, espectro de absorção no infravermelho, diagrama de raios-x, análise por microscopia de reflexão e análise por microssonda eletrônica, confirmando a presença de fosfomolibdato de amônio na estrutura do grão da resina. Estudaram-se, em seguida, as melhores condições de retenção de césio em coluna de R-FMA, hem como sua eluição. Foram igualmente investigadas as contaminações de alguns produtos de fissão polivalentes, tais como rutènio, terra* raras e zircònio na scipção de césio-137 em coluna de R-FMA, em meio ácido. Aplicou-se este trocador na recuperação seletiva de césio-137 das soluções de urânio irradiado. Destaca-se ainda a aplicação do R-FMA na preparação de uma fonte geradora de l37m Ba (2,6 min), de importância didática na determinação de meia-vida. REFERENCES* 1. ALLISON, G. M.; FERGUSON, R. A.; McLAUGHLIN, D. Chalk River, Ontario, Atomic Energy of Canada Ltd., (AECL-14148) 2. CALE'i KA, R. & KONECNY, C. Adsorption properties of ammonium molybdophosphate supported in pores of silica gel. Radiochem. Radioanal. Lett, 12:325-9, DOLEZAL, J.; STEJSKAL, J.;TYMPYL,M.; KOURIM, V. Improved inorganic ion-exchangers. II. Amonium molybdophosphate silica gel system. J. Radioanal. Chem., 21:381-7, DUTTA ROY, S. & SANKAR DAS, M. Studies on the cation-exchange behaviour of ammonium 12-Molybdophosphate. Analytica chim. Acta, 51:509-15, HIGGINS, I. R. Radiation damage to organic ion-exchange materials. Oak Ridge, Tenn., Oak Ridge National Lab., (ORNL 1325). (") Bibliographic references related to documents belonging to IPEN Library were revised according with NB-66 of ABNT.
15 11 6. HORIOKA. M. Basic studies on the separation and recovery of 137 Cs from radioactive wastes-using zeolite. Nippon Genshiryoku Gakkai-shi. 11:406-16, KRAUS, K. A.; CARLSON, T. A.; JONSON, J. S. Nature (London). 122:1128, KRTIL, J. Ion exchange properties of vanadium ferrocyanide. II. Dynamic experiments. J. Chromat. 21:85-91, LEWIS, R. E.; BUTLER, T. A.; LAMB, E. An aluminosilicate ion exchanger for recovery and transport of l37 Cs from fission-product wastes. Nucl. Sri. Engng, 2^:118-22, RIBAS, F. J.; ABRÂ0, A.; LIMA, F. W. Concentration and purification of cesium-137 from fission products. São Paulo, Instituto de Energia Atômica, dez (IEA-Pub-109). 11. SMIT, J. van R. Ammonium salts of the heteropolyacids as ca.ion exchangers. Nature (London), 1 1(4682):1530-1, May SMIT, J. van R. & JACOBS, J. J. Separation of cesium from fission product wastes by ion exchange on ammonium molybdophosphate. Ind. Eng. Chem., Process Des. Dev., 5(2) :117-22, Apr SMIT, J. van Ft.; ROBB, W.; JACOBS, J. J. AMP. effective ion exchanger for treating fi.sion waste. Nucleonics, 12(9) :116-23, Sept SMiT, J. van R.; ROBB, W.; JACOBS, J. J. J. inorg. nucl. Chem.. i :104, STEJSKAL, J.; SOUKUP, J.; OOLEZAL, J.; KOURIM, V. Improved inorganic ion-exchangers. I. Systems with organic polymers as binding materials. J. Radioanal. Chem., 21:371-9, VEROT, J. L; BLUM, J. M.; SAREATI, R.; DAGNES, J.; CASSIN, Y. Decontamination des ef'luents par les zeolithes. Bruxelles, Communaute Europeenne de L'Eenergie Atomique, 1967 (CUR-3452f).
16 INSTITUTO DE PESQUISAS ENERGÉTICAS E NUCLEARES Caixa Postal, Pinheiros CEP SSo Paulo - SP Telefone: Endereço Telegráfico - IPENUCLEAR Telex - (011) IPEN - BR